the hardening and softening of human tooth enamel
Post on 30-Sep-2016
Embed Size (px)
Australian Dental Journal, June, I968 219
The hardening and softening of human tooth enamel
B. Lilienthal,* D. H. Napper,t and B. M. Smythet
Many studies(') have shown that the hydroxy- apatite in tooth enamel exists in dynamic equi- librium with i t s fluid environment. As one of the early stages in the formation of a carious lesion involves the demineralization of tooth enamel it is apparent that a n agent which can reduce the rate of dissolution of hydroxy- apatite may have some retarding effect on the progress of dental caries.
It i s obvious that changes in the concentra- tions of calcium and orthophosphate ions in solution will alter the degree of over- or under- saturation of the solution at a given pH with respect to the solid hydroxyapatite phase. Thus the addition of calcium or orthophosphate ions to buffered acidic solutions can decrease the rate of demineralization of tooth enamel. This may be at least one of the mechanisms whereby salts containing these ions have been found@) to inhibit dental caries when added to the diet of laboratory animals. In addition, we have described in previous the in-
* Formerly, School of Microbiology, University t Formerly, C.S.R. Research Laboratories, East
t: C.S.R. Research Laboratories, East Roseville,
N.S.W. Received for publication, October, 1967.
(1) Koulourides, T.--The dynamics of tooth sur- face-oral fluid equilibrium. I n Advances in oral biology (P. H. Staple, ed.). New Pork, Academic Press, Vol. 2, 1966 (pp. 149-171).
(2) Nizel, A. E., and Harris, R. S.-The effects of phosphates on experimental dental caries : A literature review. J. D. Res., 43: Supp. 6, 1123-11 3 6 (Nov.-Dec.) 19 64.
(3)Brady B. H. G . Napper D. H., and Smythe. B. M.-The diisolution ' kinetics of hydroxy- apatite. Nature, 212: 5057, 77-78 (Oct. 1) 1966.
(') Napper, D. H., and Smythe, B. M.-The dissolu- tion kinetics of hydroxyapatite in the presence of kink poisons. J. D. Res., 45: 6, 1775-1783 (Nov.-Dec.) 1966.
hibiting effect of various organic and condensed inorganic phosphate anions on the kinetics of dissolution of hydroxyapatite. The evidence indicated that these ions do not alter the equilibrium solubility of hydroxyapatite but retard the rate of dissolution of hydroxyapatite by a kink poisoning mechanism. This sug- gests a t least one mechanism whereby these phosphates may inhibit dental caries, as they have been shown to do in both and human@' tests.
If retardation of the demineralization of tooth enamel can inhibit dental caries then it is also likely that the opposing reaction of the equilibrium, remineralization, can also influence the progress of a carious lesion. Koulourides, Cueto and Pigman") have shown that it is possible to reharden the surface of tooth enamel which has previously been softened by demineralization in a n acidic buf- fered solution. The solutions which they used to reharden the enamel were metastable solu- tions, supersaturated with calcium ions and orthophosphate ions with respect t o the solid hydroxyapatite phase. The evidence suggested that the rehardening was due to some re- mineralization process.
220 Australian Dental Journal, June, I968
ing paper, then 3/0 and 4/0 grit emery polishing paper). The final buffing was by a soft polishing cloth.
We have carried out experiments lar lines and i t is the purpose of to present these results.
along simi- this report
Materials and methods Knoop hardness scale
"he technique for measuring the hardness of dental enamel is essentially identical with that used for testing the hardness of certain metal- lurgical specimens. Indeed, human dental enamel is comparable in hardness to that of a hard stainless steel.(*)
The hardness of enamel is related to the depth of penetration of a n indenting diamond into the enamel surface for constant energy expenditure. The harder the enamel, the less is the distance of penetration. The indenting diamond is fashioned so that the area of inden- tation is proportional to the distance of penetration.
A Knoop diamond produces a diamond- shaped indentation with a n axial ratio of about 7 : l . The Knoop hardness number (KHN) is deflned as the ratio of the applied load ( in kilograms) to the area of indentation (in square millimetres) using a Knoop diamond.
P r q a r a t i o n of teeth The teeth were predominantly posterior
(both maxillary and mandibular) but about 20 per cent were anterior. Most of the posterior teeth were molars. The teeth were sectioned to obtain lingual, buccal, mesial, distal or labial surfaces. Previous workers have shown that different surfaces were of comparable hard- n e s ~ . @ ) ( ~ ) The teeth were stored in water with thymol crystals to reduce both dehydration and bacterial attack.
Each tooth section was mounted onto a poly- methylmethacrylate block, the base of which had been machined flat. This mounting was achieved using a methacrylate glue (poly- methylmethacrylate chips dissolved in chloro- form).
A small area of enamel was then ground flat and parallel to the base of the mounting block by means of increasingly fine grits of silicon carbide and emery polishing paper (progres- sively 400 and 600A grit silicon carbide grind-
("J Caldwell, R. C., Muntz, M. L., Gilmore, R. W.. and Pigman, W.-Microhardness studies of intact surface enamel. J. D. Res., 36 : 5, 732-
Test procedure The Leitz Miniload hardness tester was
employed to measure the original Knoop hard- ness of the flat, polished enamel surface. Three to five indentations only were made. The test load on the diamond was 200 g.
The enamel surface was then softened in lO-*M acetate buffer at pHz5.5 (10-8M with respect to both potassium acetate and acetic acid) for four hours without stirring. After removal from the buffer, the teeth were washed and stored in double distilled water overnight (about 15 hours). The decrease in hardness of the enamel was ca. 100-150 Knoop hardness numbers. This large decrease was necessary i n order t o blanket the considerable variation in the hardness of the tooth surface (upwards of 50 Knoop hardness units), even over a small area.
Initially the indentations were placed in a row so that the rehardening indentations could be placed adjacent. However, the considerable variation in enamel hardness rendered this method rather suspect. Consequently a n alterna- tive procedure was adopted. This involved scattering the indentations over a suitable area of surface and placing the rehardening indentations between these original indenta- tions. This procedure proved more satisfactory. The initial hardness thus involved about 20 measurements ; subsequent hardness values during rehardening each involved four indenta- tions scattered over the area.
Toothpaste experlments Toothpastes were prepared containing 0, 5,
10 and 20 per cent calcium sucrose phosphate (CaSP). The same ingredients were used in all cases but their relative proportions were varied to produce pastes of satisfactory con- sistency. The abrasive was dicalcium phosphate which was present in amounts ranging from 50 per cent when no CaSP was present, to 10 per cent when 20 per cent CaSP was present. Water varied from about 20 per cent with no CaSP present, to about 60 per cent when 20 per cent CaSP was present. The other basic ingredients, the concentrations of which did not vary appreciably, were sorbitol, glycerol, sodium lauryl sulphate, ethyl parahydroxy- benzoate, carrageenan, saccharin and flavouring.
Australian Dental Journal, June, 1968 22 I
Sodium fluoride and stannous fluoride were used in some toothpastes where indicated.
The toothpastes were diluted with water and dispersed by a combination of mechanical and ultrasonic agitation. Dispersion factors were determined after teeth cleaning experiments: four subjects cleaned their teeth and the total volume of saliva and water which each used was measured. Dispersion factors from 1 g. of toothpaste with 2 ml. of saliva (1:2) to 1 g. of toothpastes with 10 ml. of saliva ( 1 : l O ) were obtained. Studies on toothpaste rehardening were conducted at two different dispersions in distilled water, namely a dispersion of 1 g. of toothpaste with 5 ml. of water (1:5), and 1 g. in 1.25 ml. (1:l-25).
Measurements were also carried out on the toothpastes diluted with saliva a t a dispersion of 1:5. The saliva was a composite sample collected from four subjects immediately before the experiments. The pH was usually about 6.5.
Further experiments on the ability of certain additives to reharden softened dental enamel when added to control toothpaste slurries have been made. These studies were performed a t a level equivalent to a toothpaste containing 10 per cent by weight of the additive. The additives were dissolved into a slurry of the control toothpaste. The pH of the slurry was adjusted with one or two drops of 1N KOH where necessary.
The teeth to be rehardened were rotated at about 325 r.p.m. in the slurry; sedimentation of the slurry particles was prevented by con- comitant mechanical agitation. At suitable intervals, the teeth were removed from the slurry, washed and their Knoop hardness determined. The indentations placed on the tooth surface prior to rehardening were also remeasured. No appreciable change in size was ever observed. Rehardening was carried out a t ambient temperatures.
In addition to these experiments on re- hardening by rotation of softened teeth in a toothpaste dispersion, the use of a n electric toothbrush was used to simulate the normal application of toothpastes. Toothbrushlng was found to remove enamel from softened sur- faces. Unsoftened tooth